48
Thermal Analysis: methods, principles, applica5on Andrey Tarasov Lecture on Thermal analysis 26.16.2012 Andrey Tarasov, Thermal analysis, Lecture series heterogeneous catalysis, FHI MPG, 26.10.12

lyduong
• Category

## Documents

• view

261

8

### Transcript of Thermal Analysis: methods, principles, applicaion

ThermalAnalysis:methods,principles,applica5on

AndreyTarasovLectureonThermalanalysis

26.16.2012Andrey Tarasov, Thermal analysis, Lecture series heterogeneous catalysis, FHI MPG, 26.10.12

Andrey Tarasov, Thermal analysis, Lecture series heterogeneous catalysis, FHI MPG, 26.10.12

Main definitions

Heat Capacity

Heat

Thermal conductivity

λ=a·Cp·ρ =[J/s/m/K]=[W/m/K]

a – thermal diffusivity, m2/s

C=Q/ΔT, [J/mol/K]

2

Defini5onofTAGroupofphysical‐chemicalmethodswhichdealwithstudyingmaterialsand processes under condi5ons of programmed changing's of thesurroundingtemperature.

r, φ - polar coordinates z - applicate λ – Thermal conductivity , J/(cm*s*K) Cp – Thermal capacity, J/(g*K) ρ– density, g/(cm3) Q – heat of the process (reaction) α – degree of conversion

Differential Heat equation

Main Thermo-physical properties of materials

Property/Characteris5cMathema5calexpression Unit Method

Thermalconduc5vity λ(T)=a·Cp(T)·ρ(T) W/(m*K) LFA

Thermallinearexpansion

ε=1/r*(dr/dT) %/K DIL

Enthalpy dQ/dt=m·Cp·(dT/dt) J/g DSC

Weight/Composi5on/Conversion

α=(mo-mi)/mo % TG

Andrey Tarasov, Thermal analysis, Lecture series heterogeneous catalysis, FHI MPG, 26.10.12

a – thermal diffusivity, cm2/s

3

Andrey Tarasov, Thermal analysis, Lecture series heterogeneous catalysis, FHI MPG, 26.10.12

Thermal conductivity, thermal diffusivity

4

Laser Flash Method (LFA)

Andrey Tarasov, Thermal analysis, Lecture series heterogeneous catalysis, FHI MPG, 26.10.12

λ(T)=a·Cp(T)·ρ(T)

5

Andrey Tarasov, Thermal analysis, Lecture series heterogeneous catalysis, FHI MPG, 26.10.12

Dilatometry (DIL)

DIL Measurement Information

• Linear thermal expansion • Determination of coefficient of thermal expansion • Sintering temperatures • Softening points • Phase transitions

ε=1/r*(dr/dT)

SiN thermal shrinkage

ε – thermal expansion coefficient r – sample length

5

PrincipleofcombinedthermocoupleRegistra5onthetemperatureoftheobjectandtemperaturedifferencebetweensampleandreference

ConsequenceDependingontheengineeringdesign,measuringcellconstruc5onandthewayofdatarepresenta5on,varietyofmethodshasbeenarisen:DTG,DTA,DSC,STAetc.

Andrey Tarasov, Thermal analysis, Lecture series heterogeneous catalysis, FHI MPG, 26.10.12

Basic Principles and Terminology

6

InACThermoLab

TA–(Thermalanalysis)TSvs.tTG–(Thermogravimetricanalysis)Δmvs.T

DSC‐(Differen5alScanningCalorimetry):VoltagetokeepΔT=TS‐TR=0vs.T

DTA‐(Differen5alThermalAnalysis)ΔT=TS‐TRvs.T

DDTA‐(Deriva5veDTA)dΔT/dtvs.T

RDTA(ReverseDifferen5alThermalAnalysis)dt/dTvs.T

STA–SimultaneousThermalAnalysis:TG–DSC;EVA–Evolvedgasanalysis:MS,FTIR,GC

Calvet TA

Hyphenated techniques

DSC-TG

TG

DTA-TG

Basic Principles and Terminology

Andrey Tarasov, Thermal analysis, Lecture series heterogeneous catalysis, FHI MPG, 26.10.12

Calvet-DSC

7

Type Composi+on Temperaturerange,K Outputvoltage(0°C),mVTmin Tmax

T Cu/constantan 3 670 20

J Fe/constantan 70 870 34

E chromel/constantan ‐ 970 45

K chromel/alumel 220 1270 41

S Pt/PtRh(10) 270 1570 13

R Pt/PtRh(13) 220 1570 12

C W/WRe(26) ‐ 2670 39

N Nicrosil/Nisil ‐ 1200 39Constantan - 58% Cu, 42% Ni

Chromel – 89% Ni, 10% Cr, 1%Fe

Alumel – 94% Ni, 2% Al, 1,5% Si, 2,5 % Mn

Nicrosil/Nisil – Ni, Cr, Silicon/Ni, Silicon

CuNi disk sensor on Ag plate.

Cu/Constantan disk sensor on Si(X) waffer.

µ sensor τ sensor

Pt-PtRh(10) diskshaped thermocouple

Basic Principles and Terminology

Thermocouples

Andrey Tarasov, Thermal analysis, Lecture series heterogeneous catalysis, FHI MPG, 26.10.12 8

TG DSC (Heat flux)

STA SMP - Measurement signal FB - Buoyancy force , f(T) mA - Mass of adsorbed gas, f(T) mSC - Mass of sample container mS - Mass of sample , f(T) VA - Volume of adsorbed gas , f(T) VSC - Volume of sample container VS - Volume of sample, f(T)

ρgas - Density of gas, f(T)

SMP • g = ((mSC + mS + mA) - (VSC + VS + VA) • ρgas) • g

FB

Basic Principles and Terminology

Andrey Tarasov, Thermal analysis, Lecture series heterogeneous catalysis, FHI MPG, 26.10.12 9

sensor sensor

sample reference

Basic Principles and Terminology

Andrey Tarasov, Thermal analysis, Lecture series heterogeneous catalysis, FHI MPG, 26.10.12 10

General Theory (Heat equation for inert material)

b – heating rate, K/min a -Temperature conductivity coefficient, cm2/s λ – Thermal conductivity , J/(cm*s*K) Cp – Thermal capacity, J/(g*K) ρ– density, g/(cm3)

r, φ - polar coordinates

Temperature lag

Andrey Tarasov, Thermal analysis, Lecture series heterogeneous catalysis, FHI MPG, 26.10.12 11

General Theory (Temperature field in active sample)

Temperatureandreac5onextentfieldforendothermicprocess

Temperatureandreac5onextentfieldforexothermicprocesses

Exothermic ΔQ>0, ΔH<0

Endothermic ΔQ<0, ΔH>0

Andrey Tarasov, Thermal analysis, Lecture series heterogeneous catalysis, FHI MPG, 26.10.12 12

Pb(S) → Pb(L), ΔH°298= 5 kJ/mol

Setup baseline (zero line)

Baseline interpolated

Endothermic peak

CuO(S)+H2(g)→ CuO(s)+H2O(g) , ΔH°298= -86 kJ/mol

DSC TG

Measurements may have a significant change in weight due to changes in gas density and viscosity.

Shift of the baseline could appear due to change in thermal resistance of the setup. Position is depending on measuring-history.

General Theory

Blank measurement (zero line)

Andrey Tarasov, Thermal analysis, Lecture series heterogeneous catalysis, FHI MPG, 26.10.12 13

Andrey Tarasov, Thermal analysis, Lecture series heterogeneous catalysis, FHI MPG, 26.10.12

Heat of the process is determined as follows:

S –availablesurfaceforheatexchangem–samplemassΔT–generatedtemperaturedifference

General Theory

A –DSCpeakarea

Heat balance Λ(T) – heattransfercoefficientc –measuringcellheatcapacityM–massofthemeasuringcellΔT–generatedtemperaturedifferenceα‐normalizedconversion

14

Standard Mel+ngPoint,°C HeatofFusion,J/g

In 156,6 ‐28,6

Sn 231,9 ‐60,1

Bi 271,4 ‐53,1

Pb 327,5 ‐23,0

Zn 419,5 ‐107,5

Al 660,0 ‐397,0

Al‐Si 577‐880 ‐

Ag 961,8 ‐104,6

Au 1064,2

Unalloeydsteels 1147‐1536 ‐

Ni 1455,0 ‐290,4

Pd 1554,8 ‐157,3

General Theory

Calibration Standards

Andrey Tarasov, Thermal analysis, Lecture series heterogeneous catalysis, FHI MPG, 26.10.12 15

Andrey Tarasov, Thermal analysis, Lecture series heterogeneous catalysis, FHI MPG, 26.10.12

1.  ExperimentalDTAcurve2.  DTAcurvecorrectedtoheattransfercondi5ons3.  TruebaselineofDTAcurve4.  Interpolatedbaseline;5.  Experimentalbaseline;6.  Experimentalbaselinealerprocess,shiledbecauseof

thermalcapacitychanges.

General Theory (DTA equation)

φ – hea/ngrate,K/min

16

DSC Artifacts

General Theory

Andrey Tarasov, Thermal analysis, Lecture series heterogeneous catalysis, FHI MPG, 26.10.12 17

General Theory

Baseline

Calibration, KDTA, τ

3 major aspects of correct DSC measurement:

Andrey Tarasov, Thermal analysis, Lecture series heterogeneous catalysis, FHI MPG, 26.10.12 18

General Theory

Baseline definition.

3 Tangential Area-Proportional Baseline This baseline is used when the melting process is accompanied by a notable Cp change and a sloping baseline exists.

2 Sigmoidal Baseline This baseline is used when the melting process is accompanied by a notable Cp change.

1 Linear Baseline It should be used for measurements in which no significant Cp changes are observed during melting. The linear baseline is generally used.

Andrey Tarasov, Thermal analysis, Lecture series heterogeneous catalysis, FHI MPG, 26.10.12 19

Au(S) → Au(L), ΔH°298= 12,6 kJ/mol In(S) → In(L), ΔH°298= 3.3 kJ/mol

sigmoidal linear

tangential Andrey Tarasov, Thermal analysis, Lecture series heterogeneous catalysis, FHI MPG, 26.10.12

General Theory

CuO/ZnAl2O4+H2 →Cu/ZnAl2O4+H2O

20

Andrey Tarasov, Thermal analysis, Lecture series heterogeneous catalysis, FHI MPG, 26.10.12

DSC peak Correction

General Theory

In(S) → In(L), ΔH°298= 3.3 kJ/mol

Issues by uncorrected data

1.  Temperature on the peak point does not correspond to the melting temperature (but from physical point of view the sample temperature should be equal to melting point)

2.  After peak maximum the signal diminishes slowly. (Although it is known that the sample is completely molten)

21

Good Thermal contact Short melting time Sharp peak

The slope of the peak left side is depended on thermal resistance Peak area is the same and equals melting enthalpy.

General Theory

Andrey Tarasov, Thermal analysis, Lecture series heterogeneous catalysis, FHI MPG, 26.10.12 22

small τ

f(t) – evolved heat F(t) – measured signal g(t) – response function

g(t)=exp(-t/τ)

The peak right side is depended on instrument time constant.

τ1 < τ2

big τ

General Theory

Andrey Tarasov, Thermal analysis, Lecture series heterogeneous catalysis, FHI MPG, 26.10.12 23

Original signal Time constant correction Full correction

Andrey Tarasov, Thermal analysis, Lecture series heterogeneous catalysis, FHI MPG, 26.10.12

General Theory

DSC peak Correction

24

Theproper5esofthesystem«sample‐sensor»stronglyinfluencetheexperimentalTAcurves

Informa5onobtaineddependsonprocedureNotfundamentalproperty

FeaturesofTASetup

a) Reac5onAtmosphereb) Sizeandshapeoftheovenc) Sampleholdermateriald) Sampleholdergeometrye) Hea5ngratef) Thermocouple(wirediameter)g) Thermocoupleloca5onh) Response5me

Characteris5csofthesample

a)  Par5clesizeb)  Thermalconduc5vityc)  Thermalcapacityd)  Packingdensityofpar5cles(powder,pill,tablet)e)  Sampleexpansionandshrinkingf)  Samplemassg)  Inertfillerh)  Degreeofcrystallinity

Andrey Tarasov, Thermal analysis, Lecture series heterogeneous catalysis, FHI MPG, 26.10.12

General Theory

25

Dehydration of CaC2O4·nH2O in an open crucible in a dry air flow (red curve) and in a static atmosphere (green curve).

СаС2О4∙nН2О→СаС2О4+nН2О→СаСО3+1/2СО2→СаО+СО21stage 2stage 3stage

Influence of external gas flow Setup:Netzsch–STAJupiter

Andrey Tarasov, Thermal analysis, Lecture series heterogeneous catalysis, FHI MPG, 26.10.12 26

Influence of external atmosphere Setup:Netzsch–STAJupiter

TG

Dr. Andrey Tarasov, Thermal analysis, Lecture series heterogeneous catalysis, FHI MPG, 26.10.12 27

Influence of external atmosphere

Ar, 100ml/min

Vacuum 10-4 bar

k1

DSC‐TGsampleholder,Sampleweight:10mg

Andrey Tarasov, Thermal analysis, Lecture series heterogeneous catalysis, FHI MPG, 26.10.12

M=CuxZn1-x

28

Influence of sample mass

k1

Andrey Tarasov, Thermal analysis, Lecture series heterogeneous catalysis, FHI MPG, 26.10.12 29

Influence of heating rate

Andrey Tarasov, Thermal analysis, Lecture series heterogeneous catalysis, FHI MPG, 26.10.12

Independent processes

Ea1<Ea2

30

Andrey Tarasov, Thermal analysis, Lecture series heterogeneous catalysis, FHI MPG, 26.10.12

Subsequent processes

Influence of heating rate

La(OH)3→LaOOH+H2O LaOOH→La2O3+H2O

31

Competitive process processes

Influence of heating rate

Ea1<Ea2

32 Andrey Tarasov, Thermal analysis, Lecture series heterogeneous catalysis, FHI MPG, 26.10.12

Influence of the pan material Setup:Netzsch–STAJupiter

Al Pt Al2O3 Ni Cu Quartz

PyrolisisofFluoropolymer:TFE‐VDF,‐{C2F4}n‐{C2H2F2}m,F42–inAlanAupans

10Kpm,Ar,100ml/min

in Al

in Au

Andrey Tarasov, Thermal analysis, Lecture series heterogeneous catalysis, FHI MPG, 26.10.12 33

Setup:Netzsch–STAJupiter

Interac5onofTaandNbwithFluoropolymer:TFE‐VDF,‐{C2F4}n‐{C2H2F2}m‐,F42

Strong exothermic reactions

ΔM

-strong heat evolution, narrow ΔT

- 2 stages by interaction - sharp weight loss due to reaction between two solid interfaces.

Mass loss: reflects the available metal surface which is in contact with polymer.

with A. Alikhanjan, and I. Arkhangelsky (2009)

Ta-F42

Andrey Tarasov, Thermal analysis, Lecture series heterogeneous catalysis, FHI MPG, 26.10.12 34

Exothermic

Endothermic (due to water traces)

Setup:Netzsch–STAJupiter

Two effects coinsides resulting in endothermic effect.

Strong exothermic reactions

35 Andrey Tarasov, Thermal analysis, Lecture series heterogeneous catalysis, FHI MPG, 26.10.12

Measurementininert.Isthesystemoxygenfree?Setup:Netzsch–STAJupiter

O2tracesof0.25ppm

CuC2O4∙0.5H2O→Cu+2CO2

DSC‐TGsampleholder,Al2O3pan,Ar100ml/minSample:CuC2O4∙0.5H2OWeight:9.1mg

Cu+1/2O2→CuO

Andrey Tarasov, Thermal analysis, Lecture series heterogeneous catalysis, FHI MPG, 26.10.12 36

Setup:Netzsch–STAJupiter

Ni+1/2O2→NiO

@RTO2tracesof1.7ppm

DSC‐TGsampleholder,Al2O3pan,Ar100ml/minSample:Ni/MgAl2O4Weight:14.1mg

Measurementininert.Isthesystemoxygenfree?

Andrey Tarasov, Thermal analysis, Lecture series heterogeneous catalysis, FHI MPG, 26.10.12 37

Setup:Rubotherm–MSB

TGsampleholder,Al2O3pan,Ar250ml/minSample:CuC2O4∙0.5H2OWeight:301.8mg

O2tracesof7ppm

Measurementininert.Isthesystemoxygenfree?

CuC2O4∙0.5H2O→Cu+2CO2

Cu+1/2O2→CuO

Andrey Tarasov, Thermal analysis, Lecture series heterogeneous catalysis, FHI MPG, 26.10.12 38

Χ=ΔНf/ΔHfo

ΔHfo = 99.3J/g

ΔHfo – enthalpy of polymer with 100% degree of crystallinity

Determina5onofcrystallinitydegree

TFE‐VDF,‐{C2F4}n‐{C2H2F2}m‐,F42

X-degree of crystallinity

39 Andrey Tarasov, Thermal analysis, Lecture series heterogeneous catalysis, FHI MPG, 26.10.12

TA-MS Coupling systems

Skimmer coupling system

40 Andrey Tarasov, Thermal analysis, Lecture series heterogeneous catalysis, FHI MPG, 26.10.12

Capillary coupling system

41 Andrey Tarasov, Thermal analysis, Lecture series heterogeneous catalysis, FHI MPG, 26.10.12

TA-MS Coupling systems

Main Problems of TA-MS coupling system

Pressure reduction 103mbar → 10-5mbar

Condensation and secondary reactions Unfalsified gas transfer Different viscosity – Demixing

Attribution of a fragment to a chemical process Pyrolysis or evaporation MS fragmentation or sample behavior

Overlapping of thermal processes hydrolysis and oxidation due to rest water and oxygen background in the feed.

Kaiserberger (1999)

Disadvantages: shock sensitive, no direct MS inlet.

42 Andrey Tarasov, Thermal analysis, Lecture series heterogeneous catalysis, FHI MPG, 26.10.12

(PulseTA®) Adsorption of Methanol on β-AlF3

TA-MS curves for a PulseTA® experiment on pretreated (2 h, 250 °C; vacuum)

Sample:β‐AlF3Sampleweight:43.81mgΔm=0.15mg,N2‐70ml/min

M. Feist et. al. 2010

Determining Lewis acidity

43 Andrey Tarasov, Thermal analysis, Lecture series heterogeneous catalysis, FHI MPG, 26.10.12

PTA curves of NiO/MgAl2O4 after reduction, isothermal at 45°C with O2 injections, Interupted by a H2 pulse

µO(chemisorbed)/µNi(reduced)=0.22

** Assuming O/Ni=2, dNi=9nm in agreement with TEM Sample:Ni/MgAl2O4

Sampleweight:30.8mgΔm=1.14mg,Ar‐100ml/min

(PulseTA®) Titration of Ni surface with O2

44 Andrey Tarasov, Thermal analysis, Lecture series heterogeneous catalysis, FHI MPG, 26.10.12

Resources

• J. Sestak, Thermophysical properties of solids (Academia, Prague, 1984)

• G. Höhne, W. Hemminger, H.-J.Flammersheim, Differential Scanning Calorimetry (Springer, Berlin, 1996)

• E. Moukhina, J. Therm Anal. Calorim. (2012) 109: 1203-1214

• http://www.netzsch.com

45 Andrey Tarasov, Thermal analysis, Lecture series heterogeneous catalysis, FHI MPG, 26.10.12

Acknowledgments

Dr. Elena Moukhina, Netzsch Gerätebau GmbH, Selb

Dr. Jan Hanss, Netzsch Gerätebau GmbH, Selb

Dr. Michael Feist, HU Berlin

Prof. Igor Arkhangelsky, MSU Moscow

Dr. Alexander Dunaev, MSU Moscow

thermal analysis

Andrey Tarasov, Thermal analysis, Lecture series heterogeneous catalysis, FHI MPG, 26.10.12 46

Thank you!

47